Materials Chemistry and Physics 135 (2012) 1064e1069
Contents lists available at SciVerse ScienceDirect
Materials Chemistry and Physics journal homepage: www.elsevier.com/locate/matchemphys
Multisite luminescence of rare earth doped TiO2 anatase nanoparticles c a, Marko G. Nikoli c a, Milena Marinovi c-Cincovi c a, Zeljka Anti c a, Radenka M. Krsmanovi a b a ,* canin Miodrag Mitri c , Stefano Polizzi , Miroslav D. Drami a b
Vinca Institute of Nuclear Sciences, University of Belgrade, P.O. Box 522, 11001 Belgrade, Serbia Università Ca’ Foscari Venezia, Dipartimento di Scienze Molecolari e Nanosistemi, Via Torino, 155b I-30172 Mestre, Italy
h i g h l i g h t s
g r a p h i c a l a b s t r a c t
< Sm3þ, Eu3þ and Tb3þ are incorporated into anatase nanocrystals via solegel route. < Sm3þ and Eu3þ luminescence originate from 3 different sites in TiO2 nanocrystals. < Details on multisite structure for Sm3þ doped TiO2 are presented for the ﬁrst time.
a r t i c l e i n f o
a b s t r a c t
Article history: Received 12 October 2011 Received in revised form 26 April 2012 Accepted 13 June 2012
Eu3þ, Sm3þ and Tb3þ ions have been incorporated into anatase TiO2 nanocrystals via hydrolytic solegel method. Pure anatase phase was conﬁrmed with XRD and TEM measurements. Band gap energies change slightly with rare earth incorporation, from 3.32 eV for undoped TiO2 to 3.15 eV, 3.25 eV and 3.29 eV for Tb3þ, Sm3þ and Eu3þ doped TiO2. Photoluminescence of Eu3þ and Sm3þ originated from three different sites in TiO2 nanocrystals have been identiﬁed with the laser-excited site-selective spectroscopy measurements at 10 K. One site exhibits broad emission peaks, which are ascribed to the distorted lattice site near the surface. Other two sites, associated with the inner lattice, show signiﬁcantly sharper ﬂuorescence lines as a consequence of an ordered crystalline environment. The emission decays of Eu3þ and Sm3þ have similar values for inner-lattice sites and longer lifetimes for near-surface sites. The luminescence of Tb3þ doped TiO2 nanocrystals was immeasurably weak. Ó 2012 Elsevier B.V. All rights reserved.
Keywords: Nanostructures Optical materials Photoluminescence spectroscopy Optical properties
1. Introduction Titanium (IV)-oxide occurs in nature in three mineral forms: anatase, brookite and rutile. All three phases are characterized with high refractive index (nanatase ¼ 2.488, nrutile ¼ 2.609, nbrookite ¼ 2.583), low absorption and low dispersion in visible and near-infrared spectral regions, high chemical and thermal stabilities. This important metal-oxide semiconductor with relatively wide band gap (3.25 eV for anatase, 3.0 eV for rutile, 1.9 eV for
* Corresponding author. Tel.: þ381 11 3408 191; fax: þ381 11 3408 607. E-mail address: [email protected]
(M.D. Drami canin). 0254-0584/$ e see front matter Ó 2012 Elsevier B.V. All rights reserved. http://dx.doi.org/10.1016/j.matchemphys.2012.06.016
brookite)  and low phonon energy (> rTi(IV) ¼ 68 pm, in octahedral coordination, data taken from www.webelements.com) into TiO2 causes the increase of the unit cell and induces disorder into the lattice. Increase of the unit cell is manifested through a very small shift of the reﬂection peaks toward smaller angles. Widening of reﬂection peaks at higher diffraction angles reveals induced lattice disorder after doping. The (1 0 5) and (2 1 1) reﬂection peaks at 2q around 54.5 , as well as (1 1 6) and (2 2 0) at around 70 , are well resolved for undoped sample (see Fig. 4) while in doped samples these peaks merge in one with more pronounced effect for larger dopant ions. It is worth mentioning that doping with trivalent rare earth ions induces charge imbalance in the TiO2 crystal structure. For the studied dopant concentration there is no traces of segregate phases that could be observed from the XRD measurements. TEM observations show that TiO2 powder has dense aggregates made up of crystalline nanoparticles of about 10e20 nm in size for the maximum dimension (Fig. 4a and b). The local crystal structure of anatase was conﬁrmed by selected area electron diffraction (SAED) technique; one SAED ring diffraction pattern with marked Miller indices of anatase TiO2 (JCPDS card no. 21-1272) is given in Fig. 4c. The ring pattern conﬁrmed that our material is polycrystalline, while the grainy appearance of rings is related to the fact that the constituent crystallites have a size of 10 nm or more. Nitrogen adsorption isotherms, presenting the amount of N2 adsorbed as a function of relative pressure at 196 C, are shown in Fig. 5. According to the IUPAC classiﬁcation  isotherms are of type IV. Speciﬁc surface area calculated by BET equation, SBET, is determined to be 25 m2 g1.
Fig. 7. a) Emission spectra of TiO2:Eu3þ measured at 10 K obtained for three sites: I (excited at 464.5 nm), II (excited at 467.6 nm) and III (excited at 468.3 nm) and b) corresponding emission decay curves.
Antic et al. / Materials Chemistry and Physics 135 (2012) 1064e1069 Z.
Fig. 8. a) Emission spectra of TiO2:Sm3þ measured at 10 K obtained for three sites: I (excited at 464.9 nm), II (excited at 477.6 nm) and III (excited at 484.6 nm) and b) corresponding emission decay curves.
The UV/vis reﬂectance spectra of undoped and RE3þ doped TiO2 nanocrystalline powders are used to estimate energy band gaps. [F(R) hn]2 versus hn (indirect semiconductor band gap) in the vicinity of absorption edge are plotted for all samples in Fig. 6. F(R) is the KubelkaeMunk function [26,27] deﬁned as F(R) ¼ (1 R)2/2R, hn is photon energy and R is measured reﬂectance. By the extrapolation of the linear part of the curve to the intersect with x-axes one can assess band gap energies of 3.32 eV for undoped and 3.15 eV, 3.25 eV and 3.29 eV for Tb3þ, Sm3þ and Eu3þ doped TiO2, respectively. The results correspond well to those reported in the literature for anatase nanoparticles . The small decrease in band gap values for rare earth doped nanocrystals may hardly be ascribed to quantum conﬁnement effect (even though reduction of particle size is evidenced after rare earth ions incorporation) since particle sizes exceed the Bohr radius by a factor of 4 . The
Fig. 9. Schematic representation of the sites II and III local environment in TiO2 anatase structure.
possible explanation could be a slight modiﬁcation of materials density of states after incorporation of trivalent rare earth ions . Photoluminescence emission properties of rare earth doped TiO2 is investigated by means of laser excited high resolution site-selective spectroscopy at low temperature (10 K) and emission decay measurements. Emission from multiple sites is evidenced for Eu3þ and Sm3þ doped samples, shown in Figs. 7a and 8a, respectively. Neglected emission is found for Tb3þ doped sample, which was expected since Tb3þ excited states have larger energy than the trap levels of anatase nanocrystals . The multisite structure of Eu3þ in anatase nanocrystals was ﬁrst evidenced by Luo et al.  and Liu et al. . However, in the case of Er3þ doped anatase only one single lattice site emission is found by the same authors . Our results on multisite emission of Eu3þ doped anatase (Fig. 7) conﬁrm reported ﬁndings in [32,33] (number of sites and site symmetries) and the same three-site structure has been proved for Sm3þ doped TiO2 sample (see Fig. 8). Photoluminescence spectra are composed of characteristic emission bands of trivalent Eu3þ (5D0 / 7F0, 7F1, 7F2, 7F3 and 7F4) and Sm3þ (4G5/2 / 6H5/2, 6H7/2, 6 H9/2 and 6H11/2) ions (see Figs. 7a and 8a). According to branching and selection rules  one may conclude that incorporation of larger ions and charge imbalance reduces site symmetry from D2d to C1 for site I, to C2v for site II and D2 for site III, for both Eu3þ and Sm3þ doped anatase nanocrystals. Emission spectra from the lowest symmetry site I are quite broadened and can be related to distorted sites near nanoparticle’s surface or other defects. Spectra from other two sites (site II and site III) are composed of sharp emission lines, suggesting a crystalline environment for rare earth ions (of strong covalency) and their incorporation into nanoparticle volume. Schematic representation of the sites II and III is given in Fig. 9. In undoped anatase both sites have similar environment, being inside the scalenohedrons, with local symmetry 42m (D2d). Titanium ion could occupy the site in the smaller scalenohedron (site III, volume 9.45 Å3) or the vacancy in the larger scalenohedron (site II, volume 13.26 Å3). After incorporation of large RE3þ ions these sites reduce symmetries (remaining in the same symmetry group) due to distortions. The environment of smaller site III takes disphenoidal geometry (D2 local symmetry), while the larger site II takes pyramidal geometry (C2v local symmetry). The PL excitation spectrum of Eu3þ and Sm3þ-doped TiO2 samples with marked transitions, measured in the spectral region between 350 and 550 nm at room temperature, are displayed in Fig. 10. In the spectrum of Eu-doped sample (Fig. 10a) four excitation bands could be identiﬁed and attributed to the direct
Antic et al. / Materials Chemistry and Physics 135 (2012) 1064e1069 Z.
Fig. 10. Excitation spectra of a) TiO2:Eu3þ (lem ¼ 613 nm) and b) TiO2:Sm3þ (lem ¼ 612 nm) measured at room temperature.
excitation of Eu3þ ions to the 5L6 (394 nm), 5D3 (415 nm), 5D2 (464 nm) and 5D1 (533 nm) levels. The excitation spectrum of Smdoped sample (Fig. 10b) exhibits the most pronounced band centered at w360 nm, associated with the band-to-band excitation of TiO2 and the following energy transfer to Sm3þ ions, indicating that the sensitized excitation is more efﬁcient than the direct one [8,31]. Other two, less pronounced excitation bands, centered at 411 and 476 nm, could be attributed to the direct excitation of Sm3þ ions to the 6G7/2 and 4I13/2 levels, respectively [8,35]. Recorded emission decays (see Figs. 7b and 8b) exhibit a pure single exponential behavior excluding the possibility of decays’ superposition from different sites. Lifetime values are found to be 0.68 ms, 0.49 ms and 0.46 ms in the case of Eu3þ and 0.71 ms, 0.40 ms and 0.31 ms in the case of Sm3þ, for sites I, II and III, respectively. It is interesting to note that emission lifetime from disordered site, both for Eu3þ and Sm3þ, is longer than lifetime from higher symmetry sites II and III. Eu3þ emission decays are slightly higher compared to the previous ﬁndings . 4. Conclusions Thermal and infrared analysis revealed the typical behavior of materials produced by solegel, with removal of residual water and solvents at lower temperatures and organic compounds at higher ones, as well as the formation of crystalline anatase phase. Purity of the anatase phase in all studied samples has been conﬁrmed through XRD measurements, and at the local level with TEM observations. The small decrease in band gap values is noted for rare earth doped nanocrystals and could be ascribed to slight modiﬁcation of materials density of states induced by rare earth ions. We did not detect any luminescence from the Tb3þ-doped sample, while characteristic red emission has been observed in Eu3þ and Sm3þ-doped samples. PL laser-excited site-selective spectroscopy measurements at low temperature provided a clear evidence of Eu3þ and Sm3þ ions incorporation into anatase matrix. For both samples the existence of three different emission centers for RE ions impurities is conﬁrmed. Acknowledgments Authors acknowledge the ﬁnancial support of the Ministry of Education and Science of the Republic of Serbia (45020).
References  R. Zallen, M.P. Moret, Solid State Commun. 137 (2006) 154e157.  V. Kiisk, I. Sildos, S. Lange, V. Reedo, T. Tätte, M. Kirm, J. Aarik, Appl. Surf. Sci. 247 (2005) 412e417.  C.C. Ting, S.Y. Chen, W.F. Hsieh, H.Y. Lee, J. Appl. Phys. 90 (2001) 5564.  R. Palomino-Merino, A. Conde-Gallardo, M. García-Rocha, I. HernándezCalderón, V. Castaño, R. Rodríguez, Thin Solid Films 401 (2001) 118e123.  A. Conde-Gallardo, M. García-Rocha, R. Palomino-Merino, M.P. VelásquezQuesada, I. Hernández-Calderón, Appl. Surf. Sci. 212-213 (2003) 583e588.  C. Urlacher, J. Mugnier, J. Raman. Spectrosc. 27 (1996) 785e792.  S. Lange, I. Sildos, V. Kiisk, J. Aarik, Mat. Sci. Eng. B-Solid 112 (2004) 87e90.  V. Kiisk, V. Reedo, O. Sild, I. Sildos, Opt. Mater. 31 (2009) 1376e1379.  C. Gao, H. Song, L. Hu, G. Pan, R. Qin, F. Wang, Q. Dai, L. Fan, L. Liu, H. Liu, J. Lumin. 128 (2008) 559e564.  C. Jia, E. Xie, A. Peng, R. Jiang, F. Ye, H. Lin, T. Xu, Thin Solid Films 496 (2006) 555e559.  M. Bettinelli, A. Speghini, D. Falcomer, M. Daldosso, V. Dallacasa, L. Romanò, J. Phys. Condens. Matter. 18 (2006) S2149.  M. Venkatachalam, V. Palanichamy, Murugesan, Mater. Chem. Phys. 104 (2007) 454e459N.  L. Li, C.K. Tsung, Z. Yang, G.D. Stucky, L.D. Sun, J.F. Wang, C.H. Yan, Adv. Mater. 20 (2008) 903e908.  F. Wu, X. Li, Z. Wang, H. Guo, L. Wu, X. Xiong, X. Wang, J. Alloys Compd. 509 (2011) 3711e3715.  D.J. Kim, S.H. Hahn, S.H. Oh, E.J. Kim, Mater. Lett. 57 (2002) 355e360.  Z. Wang, U. Helmersson, P.O. Käll, Thin Solid Films 405 (2002) 50e54.  D. Grosso, P.A. Sermon, Thin Solid Films 368 (2000) 116e124.  Z.W. Zhao, B.K. Tay, S.P. Lau, G.Q. Yu, J. Cryst. Growth 268 (2004) 543e546.  A. Bendavid, P.J. Martin, Å. Jamting, H. Takikawa, Thin Solid Films 355e356 (1999) 6e11.  E. Setiawati, K. Kawano, J. Alloys Compd. 451 (2008) 293e296.  G. Dagan, M. Tomkiewicz, J. Phys. Chem. 97 (1993) 12651e12655.  G. Socrates, Infrared and Raman Characteristic Group Frequencies - Tables and Charts, third ed., J. Wiley & Sons, Chichester, 2001.  F.B. Li, X.Z. Li, M.F. Hou, Appl. Catal. B Environ. 48 (2004) 185e194.  V. Stengl, S. Bakardjieva, N. Murafa, Mater. Chem. Phys. 114 (2009) 217e226.  K.S.W. Sing, Pure Appl. Chem. 57 (1985) 603e619.  L. Yang, B. Kruse, J. Opt. Soc. Am. A 21 (2004) 1933e1941.  L. Yang, S.J. Miklavcic, J. Opt. Soc. Am. A 22 (2005) 1866e1873.  N.D. Abazovi c, M.I. Comor, M.D. Drami canin, D.J. Jovanovi c, S.P. Ahrenkiel, J.M. Nedeljkovi c, J. Phys. Chem. B 110 (2006) 25366e25370.  U. Hörmann, U. Kaiser, M. Albrecht, J. Geserick, N. Hüsing, J. Phys. Conf. Ser. 209 (2010) 012039.  M.G. Brik, I. Sildos, V. Kiisk, Physica B 405 (2010) 2450e2456.  K.L. Frindell, M.H. Bartl, M.R. Robinson, G.C. Bazan, A. Popitsch, G.D. Stucky, J. Solid State Chem. 172 (2003) 81e88.  W. Luo, R. Li, G. Liu, M.R. Antonio, X. Chen, J. Phys. Chem. C 112 (2008) 10370e10377.  Y. Liu, W. Luo, H. Zhu, X. Chen, J. Lumin. 131 (2011) 415e422.  J.C.G. Bünzli, V. Eliseeva, in: P. Hänninen, H. Härmä (Eds.), Lanthanide Luminescence: Photophysical, Analytical and Biological Aspects, Springer-Verlag, Berlin Heidelberg, 2011, p. 39.  E. De la Rosa-Cruz, L.A. Diaz-Torres, P. Salas, R.A. Rodriguez, G.A. Kumar, J. Appl. Phys. 94 (2003) 3509e3515.